# physical chemistry of surfaces - engr. chemistry of surfaces.pdf physical chemistry of surfaces...

Post on 23-Jan-2020

3 views

Embed Size (px)

TRANSCRIPT

Physical chemistry of surfaces Nanostructures possess a large fraction of surface atoms per unit volume. The physical and chemical properties of surfaces have great importance when describing general properties of nanostructured materials. To illustrate this let us consider 1 cm3 of iron. The percentage of surface atoms will be approximately 10-5 %. When the volume in broken into smaller cubes with side 10 nm the percentage of the surface atoms would increase to 10%. To illustrate that Figure 1 shows the percentage of surface atoms changes with the cluster size for the case of Palladium clusters. The total surface energy increases with the overall surface area, which is in turn strongly dependant on the dimension of the material. One challenge in nanomaterial fabrication is to overcome the surface energy, and to prevent the nanostructure from growth in size driven by the reduction on overall surface energy. In order to stabilize the nanomaterial structures it will be necessary to understand the chemistry and physics of the surface, which represents a large percentage of the nanostructures. Surface Energy Atoms or molecules in the surface has fewer nearest neighbors and thus have dangling bonds exposed to the surface. These surface dangling bonds produce a inwardly directed force and the distance between the surface atoms/molecules and the sub-surface atoms is smaller than the distance between atoms in the bulk (interior atoms). When the particles are very small this difference in distance becomes significant and the lattice constant of the solid shows an appreciable reduction. The extra energy possessed by the surface atoms is described as the surface free energy or surface tension. The surface energy γ is by definition the required energy to create a unit area of “new” surface. For example, consider the case of figure 2. A rectangular solid is separated into two pieces. On the new created surfaces the atoms will be located in an asymmetric environment and will move towards the interior due to the breaking of the bonds at the surface. An additional force will be necessary to move the surface atoms back to its original position. The energy required per atom will be equal to the number of broken bonds Nb multiplying by

Figure 1

Figure 2

half of the bond strength ε. Therefore the surface energy is given by:

1 2 b a Nγ ε ρ=

where ρa is the surface atomic density. This is a crude model that gives a first approximation. It does not consider the interaction with higher order neighbors nor entropic or pressure-volume contributions. Nevertheless it gives in a first approximation a value for the surface energy. When there is a surface relaxation as atoms moving inwardly, or a surface restructuring surface energy will be smaller. Let us take an elementary crystal with a facet centered cubic structure (FCC) as shown in figure 3. In the facet {100} the atoms have a coordination number (this is the number of neighbors) equal to 12. Each surface atom in the {100} facet will have 4 broken bonds and the surface energy for the {100} surface will be

100 2 2 1 2 44 2 a a

εγ ε= =

Similarly each atom in the {110} surface has 5 broken chemical bonds and the atoms in the {111} surface have 3. Thus

110 1112 2 5 2 3 2 a a

ε εγ γ= =

For a given surface with a fixed surface area, the surface energy can be reduced through:

i- Surface relaxation: surface atoms or ions move inwardly ii- Surface restructuring combining the dangling bonds into new chemical bonds iii- Surface adsorption (physical or chemical) iv- Segregation or impurity enrichment through solid state diffusion

Let us consider atoms located in the surface of an atomic flat {100} surface in a cubic structure. The surface atoms are linked with one atom directly beneath and four surrounding in the surface. Each chemical bond acts as an attracting force so all the surface atoms are under the influence of a net inwardly force. Under this force the distance between the surface atoms and the sub-surface atomic layer will be smaller than

Figure 3

the distance between two atomic layers in the bulk. Furthermore, the surface atoms may also shift laterally relative to the surface atomic layer. Figure 4 shows schematically this effect. For bulk materials the effect of reduction in the dimension of the crystal lattice is very small and can be neglected, but in nanometer size structures can become important. This effect was observed in CdS nano-crystals through a significant decrease in the melting temperature relative to the bulk material. From these data it is possible to derive the corresponding decrease in the lattice parameter. Figure 5 shows plots revealing this effect. On the left the intensity of the electron diffraction of the {111} peak shows a sharp decay at decreasing temperatures for decreasing nanoparticle size, indicating the loss of the crystalline structure. On the right the lattice parameters for two different species of nanocrystals also decreases with the decreasing nanocrystal radius. Another possibility to minimize the surface energy is through a rearrangement of the surface. For example this restructuring of the

surface is found in Si crystals. In Si and diamond, the restructured {100} surface has the minimum surface energy as compared with the other lower index structures. This restructuring of the free bonds in the surface can have a significant impact in crystal growth. Figure 6 is a scheme showing this effect. At the level of individual nanostructure there are two approaches to the reduction of the total surface energy. One is to reduce the overall surface assuming that the material is isotropic. Water on a hydrophobic surface always forms spherical droplets. Amorphous materials with isotropic surface energy always reduce the overall surface energy by reducing the total surface. However for crystalline materials different facets have different energies and a crystalline particle normally forms facets instead of having an spherical shape. The thermodynamically equilibrium shape of a crystal can be determined by considering the surface energies of all facets. The final surface shape corresponding to

Figure 4

Figure 5

the minimum surface energy is obtained when different facets are combined to have an overall minimum value of the surface energy. A systematic way to determine this minimum energy surface is considering a Wulff plot. For an equilibrium crystal, ie the total energy reaches minimum, there exists a point in the interior such that its perpendicular distance hi from the ith face is proposrtional to the surface energy γi. i iC hγ = where C is a constant equal for all the surfaces. Considering this, a Wulff plot can be constructed with following steps:

i) given a set of surface energies for the various crystal faces, draw a set of vectors from a common point of length proportional to the surface energy and direction normal to that the crystal face.

ii) construct the set of faces normal to each vectors and positioned at its end, and iii) find a geometric figure whose sides are made up entirely from a particular set

of such faces that do not intersect any of the other planes

Figure 7 schematically shows a hypothetical 2 dimensional crystal with (10) and (11) planes and the final crystal surface obtained with this construction method. The three steps indicated above correspond to the three steps in the construction shown in the lower part of the figure. It should be pointed out that this type of constructions corresponds to a mathematical ideal situation, i.e. the crystal reaches the minimal surface energy level thermodynamically. In practice however the geometric figure of a crystal depends on the dynamics in the synthesis or growth conditions. Different morphologies are obtained for different processing conditions.

Figure 7

Figure 6

Chemical potential as a function of the surface curvature The properties of surface atoms or molecules are different from that of interior atoms, due to the fewer number of bonds in the surface. The chemical potential is also dependent on the curvature of the surface, so it is an important aspect to consider in nanoparticles where the radius of curvature of the surfaces are extremely small. To see that let us consider the example of figure 8. Suppose we transfer material from an infinite flat surface to a spherical solid particle. This amount of material transferred is composed by dn atoms, and the radius of the solid particle is R. The volume change of the spherical particle, dV, is equal to the atomic volume Ω times dn. That is 24dV R dR dnπ= = Ω The work per atom transferred, ∆µ, equals to the change of the chemical potential, and is given by

8c dA R dR dn dV

µ µ µ γ π∞ Ω

∆ = − = =

cµ and µ∞ are the chemical potential on the particle surface and on the flat surface respectively. Combining the two former equations

2 R

µ γ Ω∆ =

This is also called the Young- Laplace equation and describes the chemical potential of an atom in a spherical surface with respect to a flat reference surface. This equation can be readily generalized for any type of curved surfaces. The last equation indicates that the chemical potential of an atom in a convex surface (positive curvature) is higher than that on a flat surface. Mass transfer from a flat surface to a convex surface results in an increase

Recommended